Loading in 2 Seconds...
Loading in 2 Seconds...
Zinc solution. Hot plate. DC Power supply. Motivation & Purpose. Results. +. -. A. V. N.W cation. anion. +. -. Ir. cathode. Anode. electrolyte. stirrer. Synthesis of ZnO nanowire. Roughness measurement. Hydrothermal Method. Experimental. Principle of Electropolishing.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
DC Power supply
Motivation & Purpose
Synthesis of ZnO nanowire
Principle of Electropolishing
Summary & Future work
IMPROVEMENT OF HEIGHT UNIFORMITY OF ZnO NANOWIRE ARRAYS BY USING
Mee Na Park 1,*, Ee-Le Shim1, Joonho Bae 3, C. J. Kang1,2, and Young Jin Choi 1 ,2**
1 Department of Physics, MyongJi University, Yongin, 449-728, Korea
2 Dept. of Nanoscience & engineering , MyongJi University, Yongin, 449-728, Korea
3 School of Materials Science and Engineering, Georgia Institute of Technology, Atlanta, GA 30332-0245, USA
◎ Applications of ZnO nanostructures
- solar cells , chemical sensors , field emitters and nanogenerators.
◎ In order to be successfully incorporated into nanodeives,
the nanowires have to be grown with a high degree of control in
To control and improve the uniformity
of heights of ZnO nanowire arrays
An aqueous solution of phosphoric acid is used as the electrolyte to planarize the top surfaces of ZnO nanowire arrays.
Applied voltage ranged from 7 to 15 V in phosphoric acid (pH 5.0).
Apparent planarizationof protruded ZnO nanowires
. Zinc solution :
Zinc nitrate hexahydrate + Hexamethylenetetramine + Deionized water
. Concentration of solution : 7.5 mM
. Temperature : 70~90℃
. Synthesis time : 6h
(CH2)6N4 + 6 H2O ↔ 4 NH3 + 6 HCHO , (1) NH3 + H2O ↔ NH3 ·H2O, (2) NH3·H2O ↔ NH4+ + OH− , (3) Zn2+ + 2 OH−↔ Zn(OH)2 , (4) Zn(OH)2→ ZnO + H2O . (5)
(a) As-grown ZnO
(b) After EP
7V , 1h , pH 5.0
※ To directly observe the morphology change when nanowires were electropolished, patterned ZnO nanowire arrays were fabricated on Si substrate, and the same regions of nanowire arrays were compared before and after the EP process.
※ SEM image of patterned
ZnO nanowire arrays
(b) Line profile
E.P condition ; 15 V , 1min , pH 5.0
(a) Typical AFM image of as-grown ZnO nanowire arrays
Bulk concentration additive species
The height variation of nanowires was reduced after EP had been performed.
In order to optimize EP conditions for the planarization of nanowire arrays, the statistical analysis of the roughness change is in progress.
Electropolishing(EP) has been conventionally used to remove a thin layer of material on the surface of a metal part.
The basic mechanism of EP is based on the differential rates of metal removal in an aqueous solution of acid. Areas of metal with high current densities are rapidly dissolved, resulting in the smoothing of metal surfaces .
EP is the electrolytic removal of metal in a highly ionic solution by means of an electrical potential and current.
 M.Al-Ajlouni and A.Al-Hamdan, J. Applied Sci. 8(10), pp.1912-1918 (2008).
 Shih-Chieh Chang, Jia-Min Shieh, Electrochemical and Solid-State Letters. 6(5), G72-G74 (2003).
 Sheng Xu, Yaguang Wei, Zhong Lin Wang*, J. Am. Chem. Soc. 130,pp.14958–14959(2008).
 M. Law, L. E. Greene, P. D. Yang, Nature Materials 4, pp. 455 , (2005).
Nano-Scale Measurement & AnaLysis Lab.